Processing, Microstructure and Mechanical ... PROCESSING, MICROSTRUCTURE AND MECHANICAL PROPERTIES...
Embed Size (px)
Transcript of Processing, Microstructure and Mechanical ... PROCESSING, MICROSTRUCTURE AND MECHANICAL PROPERTIES...
PROCESSING, MICROSTRUCTURE AND MECHANICAL PROPERTIES OF
PM GAMMA TITANIUM ALUMINIDES
C. F. Yolton 1 , Ulrike Habel
1 and Young-Won Kim
1 Crucible Materials Corporation, 6003 Campbells Run Road,
Pittsburgh, PA 15205-1022 USA 2 UES Inc., 4401 Dayton-Xenia Road, Dayton, OH 45432-1894 USA
Keywords: TiAl, Powder, HIP
Gamma titanium aluminide alloys (TiAl) are receiving increasing attention as candidates for
advanced structural materials in high temperature aerospace applications. Inert gas atomization
of prealloyed powder followed by hot isostatic pressing (HIP) to full density is a viable
approach for the production of forging and rolling performs as well as as-HIP components.
The prealloyed powder metallurgy (PM) production route has the capability of producing a
uniform and fine microstructure in preforms/components of any size. This paper will describe
gamma titanium aluminide powder production, processing and characterization. Alloys such as
Ti-48Al-2Nb-2Cr, Gamma Met (Ti-46.5Al-4(Nb,Ta,Cr,B), and 395MM (Ti-46Al-4(Nb,Mo,Cr,
B,C) have been produced in quantities exceeding 500 kg. Microstructure and processing of
consolidated material will be discussed. Thermally induced porosity (TIP) is a phenomenon,
which occurs in any inert gas atomized powder. The results of a study to evaluate the effect of
processing and heat treatment conditions on the microstructure and occurrence of TIP in
gamma titanium aluminide powders will be presented. Mechanical properties of consolidated
product will also be presented.
Titanium aluminide alloys based on the TiAl intermetallic compound have attractive properties
particularly for structural applications in high performance aircraft and automotive engine
components as well as other applications [1,2]. The primary advantages of titanium aluminide
alloys are low density, high strength to weight ratio at elevated temperatures, a higher modulus
than conventional titanium alloys and good oxidation resistance. While gamma titanium
aluminide alloys have several attractive properties industrial scale ingot production and
wrought processing of these alloys has proven to be challenging. Some of the quality issues
related to production of large ingots are centerline porosity and pipe, grain size variations and
regions of varying density related to melt homogenization . Powder metallurgy (PM) offers
the potential for minimizing many of the problems associated with large ingot production and
the potential for reducing overall cost of the final component. Another advantage of the PM
process is that it may enable the development of alloys that cannot be made by conventional
ingot metallurgy. Gas atomization of prealloyed powder followed by hot isostatic pressing
(HIP) or consolidation by extrusion to full density is a viable approach for the production of
forging and rolling performs, as-HIP components and extruded shapes. This paper will
Niobium for High Temperature Applications
Edited by Young-Won Kim and Tadeu Carneiro
TMS (The Minerals, Metals & Materials Society), 2004
describe the prealloyed PM process for production of gamma titanium aluminide and
characterization of the product.
Powder Production and Processing
A schematic of the system developed by Crucible  for production of prealloyed gas
atomized titanium powder is shown in Figure 1. This system consists of a melting chamber, an
atomization tower and a cyclone collector. The starting charge material is melted in a cold wall
induction crucible within the melt chamber. The cold wall induction crucible is shown in
Figure 1. Titanium gas atomization system.
The starting stock for melting may be virgin raw materials or clean prealloyed stock such as
ingots or bars. As in conventional vacuum induction melting, no special preparation of the
melt stock is required. As the charge is melted a skull forms at the crucible bottom and wall so
the molten charge is always contained in a solid skull of the same composition. After the
charge is fully molten it can be held in the molten state for an extended period to assure
complete homogenization of the melt. The active stirring produced by the induction field and
the ability to hold the metal in the molten state for an extended time are particular advantages
of this type of melting system. After the starting charge is fully melted it is bottom poured into
a heated graphite susceptor. The pour is controlled by the power applied to the inductively
heated graphite susceptor and the primary power applied to the crucible. The bottom of the
susceptor contains a nozzle which forms, nominally, a 4mm (0.160inch) diameter stream that
free falls into high pressure argon gas jets which atomize the molten stream. For gamma
titanium aluminde alloys the nozzle material is typically high quality graphite. The atomization
gas carries the powder to the cyclone where the powder is collected in a removable canister.
After cooling under inert gas to room temperature, the powder is removed for further
Figure 2. Bottom pour 45kg cold
wall induction crucible.
Powder cleanliness is an important consideration in any powder that is to be used in aerospace
applications or other fatigue critical applications. This aspect has been taken into consideration
in design of the atomization system. The atomization tower is constructed entirely of stainless
steel and all internal surfaces of the tower, which may come in contact with the powder, are
polished. The atomization tower, transfer piping and cyclone collector are made up of multiple
sections joined by O-ring flanges to permit disassembly and thorough cleaning of all internal
surfaces. The cleaning is done whenever the alloy is changed to prevent cross contamination of
alloys. The atomization tower and all sections of the atomizer below the melt deck are
contained in a positive pressure room with a dedicated air handling system to prevent air borne
contamination from the general shop atmosphere.
Two processing rooms are located adjacent to the atomization tower room. These rooms
contain powder processing equipment such as screeners and blenders. The rooms are under
positive pressure with dedicated air handling systems. In addition to operations such as
screening and blending, all loading of containers for shipment or consolidation are done in
these rooms. Only one alloy is processed in a room at any time and before another alloy is
processed the equipment and the room are thoroughly cleaned.
Approximately 40 different gamma titanium aluminide compositions have been made in the
atomizer to date. Several of these alloys are listed in Table I. The majority of the alloys have
been proprietary compositions made for outside customers. Approximately 5445 kg (12,000
lbs) of gamma titanium aluminide powder have been produced in the last five years. The
estimated annual capacity of the atomizer is 4,990 to 27,223 kg (11,000 to 60,000 lbs)
depending on the number of shifts it is operated.
Table I. Gamma Titanium Aluminide Compositions
Produced by Gas Atomization
Gamma Met (Ti-46.5Al-4(Nb,Ta,Cr,B) at%
K5 (46.2Al-3Nb-2Cr-0.2W-0.2B-0.2C at%)
395MM (Ti-46.2Al-4(Cr,Nb,Mo,B,C) (at%)
More than 30 proprietary compositions.
Control of chemical composition is another important consideration in any powder making
operation. Typical chemistry tolerances for gamma titanium aluminide powder are
given in Table II.
Some alloys, such as K5 and 395MM require higher levels of carbon in the alloy. For these
alloys, carbon is added to achieve the required carbon level. In melting and atomization there is
Table II. Typical Chemistry Tolerances For Gamma Ti Aluminide Powder
Element Wt % At %
Aluminum + 0.50 + 0.56
Minor + 0.25
Iron 0.08 max
Oxygen 0.08 max
Nitrogen 0.02 max
Carbon 0.05 max
Hydrogen 0.005 max
essentially no increase in carbon, nitrogen or hydrogen over the starting melt stock. The
increase in oxygen content over the starting melt stock is typically 100 to 200 wppm for –100
Figure 4. Size distribution of gas atomized gamma titanium aluminide powder.
After atomization, a full chemistry is determined on each heat and physical properties such as
size distribution, tap density and flow rate are determined. The powder is then screened to the
required particle size. After screening the powder is loaded into suitable containers for
consolidation, outgassed, and sealed under vacuum.
Typical methods for consolidati